Macromolecules 1993,26, 61556163
6155
Reaction Kinetics Analysis of Urethane Polymerization to Gelation B. Liu,t H. Noureddini,*J. S. Dorsey,* and D. C. Timm'J Calter Services Corporation, Dallas, Texas 75261 9500, and Department of Chemical Engineering, University of Nebraska, Lincoln, Nebraska 685880126 Received January 25, 1993; Revised Manuscript Received May 24, 1 9 9 P ABSTRACT: A chemical reaction analysis of a thermosetting, urethane resin formulated from a triol and a diisocyanate is reported. Population densitydistributionsof oligomericmolecules, monomer concentration, the cumulative molar concentration of intramolecular bonds, the resin's average molecular weights, and extent of reaction were determined as a function of time. Rate expressions for intermolecularreactionswere first order with respect to the concentration of each reactant and were proportional to the functionality of their respective chemical moieties. Rate expressions for intramolecularreactionswere first order with respect to the concentrationof the reactant and were proportionalto the functionalityof the limitingchemical moiety on the reactant. The initial ratio of the chemical equivalentsand effects of dilution were incorporated into numerical simulations. Stanford and Stepto's experimental data were analyzed. Gel points and the concentration of intramolecularbonds were correlated as a function of conversion. Intramolecular reaction rate expressions derived with the aid of Gaussian chain statistics require the molar concentrations of all chemical isomers of a specified chemical composition. The present reaction rate expression allows chemical isomers to be lumped into a single population density distribution variable, substantially reducing the dimensionsof the simulation. Numerical results demonstratethat the simplified rate expressionis an excellent approximation.
Introduction The current research explicitly addresses competing intermolecular and intramolecular polymerization reactions with multifunctional monomers. The approach is based on classic chemical reaction kinetics. A major objective was the development of a meaningful, simplified rate expression for intramolecular reactions which would not explicitly require populations of the numerous chemical isomers at specified chemical compositions. The selected rate expression is proportional to the limiting chemical moiety on the reacting molecule and to the molar concentration of similar molecules. Simulations are presented that indicate the approach is accurate for a random, stepgrowth reaction on molecules with flexible chains. For a thermosetting, polyurethane, the number of intramolecular bonds as a function of conversion correlate with experimental measurements. Gel points are accurately predicted. Simulations and experiments incorporated the effects of initial ratios of the chemical moieties and the effects of dilution. Linear/Cyclic Chains. Theoretical polymerization models explicitly descriptive of intramolecular reactions have been developed for linear molecules. Theoretical foundations were developed by Jacobson and Stockmayer2 who assumed that molecules were distributed according to the most probable distribution3p4and that ring formation was dependent on Gaussian chain statistics. Semlyen5 reviewed methods for calculating the concentration of cyclicchains, including the rotational, isomeric state model developed by Flory, Crescenzi, and Mark, direct computation methods of Fluendy? Carmichael and Kinsinger,lo Semlyen,ll and Winnik et a1.12 Flory et al.1315 and Mutterl6 continued the advancement by addressing the direction of terminal bonds in coiled chains. Equilibrium data for the resins poly( 1,3dioxolane), poly(decamethylene adipate), and poly(dimethylsi1oxane)were discussed. For the larger rings, theoretical calculations correlate with + Caltex Services Corp. t University of Nebraska. Abstract publishedin Advance ACSAbstracts, October 15,1993. Q
experimental measurements. For kinetically controlled ring closure, Gordon and Scantlebury17expressed the relative kinetic rate constant in terms of the mean bond length I
The molecular weight of the repeat unit is denoted by M, initial molar concentration of the monomer by CO, chemical functionality by f , Avogradro's number by N , density by d , the valence angle by 4, and the number of atoms in the smallest ring by v. Stepto and Waywellla observed the fraction of rings as a function of conversion for a polyurethane polymerized from bifunctional monomers. Gordon and Templelganalyzed these data using chemical reaction methodology. Intermolecular reactions were first order with respect to the molar concentration of each reactant (second order overall) and were proportional to the product of the chemical functionalityon eachreactant. Intramolecular reaction rate expressions for a ring of size iv equaled k g / ( k a ( ~ i ) ~ / ' ) L Degree i. of polymerization of the cyclic chain is i. The molar concentration of the linear reactant is Li. Subject to an initial ratio of the isocyanate/hydroxyl moieties, the apparent rate constant was observed to be a function of dilution. The authorslgevaluated the relative rate constant by achieving the best fit of all observations for each experiment. They noted that benzene is a relatively poor thermodynamic solvent. An increase in solvent concentration may cause a corresponding reduction in the dimension 1 which alters the rate constant's value. Stanford et dZ0 also analyzed Stepto and Waywell's data using the FrischKilb modificationz1 of the JacobsonStockmayer theory for the prediction of gel points. Emphasis of the regression was placed on initial conversion intervals during which time the smallest sized ring was most likely to form. The authors also noted that values for 4 = go", 1 = b varied with dilution and suggested that dilution could effect the distribution of ring sizes that form. For linear polymers the variable b is known to
00249297193122266155$04.00/0 0 1993 American Chemical Society
6156 Liu et al.
increase with molecular weight. This factor would effect theoretical estimates of the number of the larger cyclic chain configurations. The linear polyurethane resins have also been analyzed with cascade theory by Gordon and Temple.2z Stepto and Waywellla also provided an analysis. Network Chains* In the area Of multifunctional monomers. Florv3and Stockmaver4Dioneered theories on gelation. Stock;;layer stated t i a t hb stochastic solution for random, stepreaction polymerizations satisfied the Smoluchowskiequation which can be derived from classic chemical reaction theory, subject to the constraint of intermolecular reactions. The resultant population density distribution yields moment equations that form conditionally convergent, infinite series with increasing conversion. Conditionally convergent series can be rearranged to converge to any limit.23i24 The difference between two selected limits of convergence for specific rearrangements was interpreted implicitly as being descriptive of the mass of the insoluble gel fraction.3 In related work, Shy and E i ~ h i n g e rused ~ ~ Monte Carlo algorithms to simulate the polymerization reported by Stanford and Stepto.26 Their model effectively calculated cyclization and gel points in bulk cures. The agreement was less than satisfactory with dilute reactions. Competing intermolecular and intramolecular reactions have been explicitly addressed. Templez7 incorporated Gaussian chain statistics into intramolecular rate expressions. The relative rate expression for a specific nonlinear molecule becomes a complex function of degree of polymerization, taking the form k,/k,C;NoJ (vi)3I2Pj. The number of ways that a ring of degree of polymerization i can form, given a specific chain configuration, is represented by No;. The molar concentration of this chemical isomer is denoted bYPj. Since the variableNo; is a function of chain configuration for moleculesof a specified chemical composition, the molar concentrations of all possible chemical isomers must be calculated. The summation accounts for competing ring closures of different dimensions. Noureddini and Timm2acontinued the development of reaction models that explicitly incorporate intramolecular reactions and sought analytical solutions for the polymerization of the multifunctional monomer RAf/&/Z. To achieve this goal the rate expression for intramoelcular reactions had to be simplified. In Semlyen's p~blication,~ data for linear/cyclic molecules are presented which show that the smallest ring formed dominates the molar concentration of cyclic molecules. Similar observations have been reported by B i l l m e ~ e for r ~ ~hydroxyl acid and amino acid polymers. A fivemember ring forms lactones or lactans exclusively, but monomers with chains containing less than five but more that seven atoms tend to form linear chains. Reactants containing six atoms in their chain form a mixture of cyclic and linear chains. Odian,30 in discussing the formation of branches in lowdensity polyethylene, also stated similar conclusions. Intramolecular chaintransfer reactions produce the low molecular weight branches. The predominant nbutyl branch as well as the 2ethylhexyl and 1,3diethyl branches form from sixmember transition states. If a proton is extracted from the sixth or seventh methylene group, namyl and nhexyl branches form. A representative lowdensity polyethylene molecule contains five nbutyl branches and one or two eachof the other branches per 500 monomer units. Subject to these observations, Noureddini and TimmZ8assumed that a specific functional group on a network molecule with relatively flexible chains will most likely react with a neighboring moiety in forming a cyclic ring configuration. The frequency of collisions between reaction sites on
Macromolecules, Vol. 26, No. 23, 1993 CH2
I
r
(OCH2CHCHz)u OH
(OCH2CHCHa),OH
n rz 17
 .
CH7(0CH2CHCH3)n ,OH
Figure
1.
Niax triol a propylene oxide adduct of glycerol.
molecules of a specific composition may be proportional to the limiting chemical functionality. The molar concentration of the reactant accounts for parallel reactions. This assumption is a first approximation of the JacobsonStockmayer theory and has been mentioned by Stepto.21 The assumption greatly reduces the dimensions of the mathematical description by allowing chemical isomers to be lumped into the dependent variable. Analytical solutions were derived for population density distributions and moments of the distribution. When data only descriptive of the moments are to be analyzed, the moment equations can be solved independently of the population density distribution dynamics which further reduces the dimensions of the problem. The present work tests the validity of this simplified rate expression for intramolecular reactions by examining experimental data. Stanford and Stepto26reported data for a polyurethane resin comprised of flexible chains. Intramolecular reactions competed with intermolecular reactions at the earliest stages of cure. The current work shows that numerical simulations accurately predict the experimentally observed extent of cyclization as a function of conversion and gel points. Experimental variants include the initial ratio of chemical equivalents and the mass fraction of resin in solution. The analysis further relates the measured relative rate constanta to fundamental parameters of the JacobsonStockmayer theory as modified by Temple.z7 The validity of the approximate rate expression was further tested by comparing numerically generated polymerization dynamics. Temple's work2' incorporated Gaussian chain statistics explicitly in network forming polymerizations. The current model satisfactorily replicates his simulations, showing that the simplified rate expression is adequate. Constrained to intermolecular reactions, numerically calculated population density distributions also replicate Stockmayer's analytical soluti0ns.3~ Experimental Section Stanford and S t e ~ t opolymerized ~~ hexamethylene diisocyanate and a propylene oxide adduct of ethyleneglycol, Niax Triol (LG56)manufacturedby Union Carbide Corporation. The triol, see Figure 1,had a molecular weight of approximately 3000. The average degree of polymerization of a branch was approximately 17. The three hydroxyls experienced equal reactivity since the size of a branch is sufficiently large to negate firstshell substitution effecbZ2The present notation considers all mol
ecules that contain at least one triol unit to be polymeric. The diisocyanate is the monomer. Polymers were prepared with an initial ratio of isocyanate equivalence to hydroxyl equivalence in the range of 1/1.5 to 1,5/1, Formulationswere prepared in the bulk and in the presence of a solvent, benzene. Dilution encourages cyclization by reducing the rate for intermolecular reactions relative to the rate for intramolecularreactions. The fraction of resin ranged from 100% to 30 % . No catalyst was present. Cures were at 70 "C. Experimentally,the number average molecular weight and the concentration of isocyanates were determined. From these data the number of intramolecular bonds within the resin was determined as a function of conversion. The gel point was determined as that conversion when the resin began to climb the shaft of the mixer. Specific details descriptive of the experiments and measurements can be found in the cited literature26 and its references.
Urethane Polymerization to Gelation 6157
Macromolecules, Vol. 26, No. 23, 1993 MONOMER
BB
PO,l,O
TRIOL
P1,o.o
diisocyanate links are required to join the iA triols into a molecule. Each link consumed two hydroxyls. The remaining isocyanates ig  (iA 1)are pendent to the chains, being connected to the molecule's infrastructure via a single bond unless they formed one of the j intramolecular links. Algebra yields the hydroxyl functionality:
A
Analogous logic yields the isocyanate functionality: A
TRIMER
A >A
BB
A
1.00
,
V."
0.5 0 4
1
0.31
i
0 21 0 14 0 054 0
0
0.1
0.2
0.3
0.4
Conversion
(PA
0.5
0.6
0.7
or PB)
lation allows this variable to be expressed explicitly as a function of the formulation parameter r, conversion P B , and the number average molecular weight MWn: (1 + 2/(3r)  2pB)MWn MW, 2MWA/(3r)
+
0'1
0'2
0'3
04
0'5
06
07
0'8
09
Conversion (PB)
Figure 3. Number fraction of ring structures as a function of conversion (r = 1, k d k l = 1, 70% solvent).
N,=l
'5
Figure 4. Number fraction of ring structures as a function of conversion of the limiting reactant (r = 111.5, k 2 / k l = 0.15,30% solvent). 0.7 I
+ Slmuktlon points
I
P
(14)
Conversion was determined experimentally by titration of the isocyanate and the number average molecular weight was determined from cryoscopic measurements.26 Initial conditions appear in Table 11. The relative rate constant kdkl was adjusted until the simulation visually fit the data. This ratio results in the independent variable k l t in the numerical program. Illustrative results appear in Figures 35 and represent the average number of intramolecular bonds per molecule, N,, as a function of conversion of the limiting functional site. Data in Figure 3 were constrained to a polymerization with equal chemical equivalents of hydroxyl and isocyanate moieties, r = 1. The formulation included 30% resin and 70% solvent. Agreement between theoretical and experimental data was realized when the relative rate constant was unity. Data of Figure 4 present similar results when excess hydroxyl moieties were present, r = 1/1.5. The solvent fraction was 30 % . Figure 5 shows representative results with an excess of isocyanate moieties, r = 1.5/1. The solvent fraction was 70%. Rate Constants. Calculated relative rate constants for several experiments are presented in Table 11. The relative rate constant is a function of dilution and is tabulated for the three sets of data at r = 1,1/1.5, and 1.5/1,respectively. The data reveal that the dependency in the relative rate constant when r = 1 and r = 1.5/1 is similar. With 70% solvent the rate constant has increased approximately 6fold compared to bulk polymerization data. Gordon and Temple22and Stepto21reported similar trends for a linear polyurethane. The relative rate constant doubled as the solution became dilute. The network resin experienced
# 0.1 0.2 0.3 0.5 0.6 0.7 I
'0
0.4
Conversion
0.8
0.9
(PA)
Figure 5. Number fraction of ring structures as a function of conversionofthelimitingreactant(r = 1.5, k d k l = 1,70% solvent). a greater number of rings and a greater dependency on solvent concentration. The data tabulated in Table I1 indicate when hydroxyl groups are in excess, r = U1.5, the relative rate constant is considerably less sensitive to solvent concentration. Gordon and Templelg observed similar findings for the linear polyurethane and stated that in a hydroxylrich environment, the "shielding of the OH groups by Hbonding might well affect differently the rate of their intramolecular and intermolecular reactions". Mean Bond Lengths. The JacobsonStockmayer theory can be interpreted, yielding the mean bond length b. The form for the intramolecular rate expression is a first approximation of the rate expression representing Gaussian chain statistics described by Temple.27 If Noi = Cia,isjand if the series in Temple's work is truncated after the initialterm, i = 1, then the relative rate constants are approximately equal, k d k l = ( k J k , ) / ( ~ ) 3 / The ~.
Urethane Polymerization to Gelation 6161
Macromolecules, Vol. 26, No. 23, 1993 relative rate constants tabulated in Table I1 yield a range in bond dimensions b of 0.130.07 nm. SteptoZ1reported a value of 0.16 nm. First approximations associated with theory likely contributed to errors, but results are approximate. Results may also indicate that current theory may have to be advanced to accurately predict the rate of cyclization in network resins. Gelation. Stanford and SteptoZ6measured the critical conversion at the gel point for several of their experiments. These data are tabulated in Table I1 if the resin gelled. For the case r = 1,dilution shifted the critical conversion to larger values, 0.7650.831. Increased levels in intramolecular bonding reduced functionalities on a reactant and consequently its rate of growth was retarded and the critical conversion increased. Data of Figure 3 show that approximately one out of three molecules contain a cyclic chain configuration at 50 %5 conversion and more than one out of two at 70%. Data in Table I1 collected with an imbalance in stoichiometry show that the critical conversion is higher due to the substantial imbalance in the concentration of functional groups and due to environmental effects. The critical conversion 0.925 with excess hydroxyls is less than the conversion a t gelation for experiments with excess isocyanates, 0.945. This fact is reflected by the values of the relative rate constants, 0.15 and 0.18, respectively. S t o ~ k m a y edeveloped r~~ an implicit theory for predicting the gel point. Subject to the constraints of intermolecular reactions, f~ = 3 and f~ = 2, the critical conversion can be estimated: (PAPB)gel
= 1/2
Therefore Estimates of the gel point based on this expression appear in Table I1 under the column labeled “eq 15”. The model does not account for functional groups consumed by intramolecular reactions and, therefore, consistently predicts gelation at lower levels of conversion. The current analysis explicitly addressed gelation. At the gel point the weight average molecular weight becomes infinite:
MWAP1,O,O(0)
h
h
5. 1204 $ I
.
9!?
0:9
1
o
B
P
E
Conversion ( p ~ )
Figure 6. Prediction of gelation cfi, = 2 , f ~= 3, r = 0.989,Po,l,o(0) = 0.454, Pl,o,o(O)= 0.306, 0% solvent). of 0.831; see Figure 3. The extrapolation to gelation resulted in a greater uncertainty, PA = 0.940. But even with this difficulty, the maximum error is only 11%. Three experiments summarized in Table I1 did not gel. Simulations indicated that two of the experiments would gel close to 100% in conversion, 0.987 and 0.995. For the third experiment, the critical gel point was predicted to exceed 100% and, therefore, one could say with a high level of confidence that gelation would not occur. In summary, the chemical reaction analysis accounted for intramolecular reactions on gelation accurately. Numerical Simulations. The present research also addressed consequences of the simplified form for the intramolecular rate expression. Temple2’ used a theoretical approach when modeling thermosetting resins. Reaction rate expressions derived for cyclization reactions of linear chains were extended to multifunctional resins. To demonstrate, consider a potential intramolecular reaction on the molecule P3,4,1 shown in Figure 2. For simplicity, the chain segments represented by lines and bonds AB are assumed to be identical with respect to their atomic structure. Each segment represented by a line is assumed to contain Y atoms. The pendent B group has an equal chance to react with each of the two A sites, making ringed chain configurations which contain six chain segments. These candidate intramolecular reactions result in the rate expression
+ MWBPO,I,O(o)
(16) The molecular weights of the two monomers are denoted by MWAand MWB. The set of differential equations that describe secondorder moments appear in the Appendix. Illustrative, numerical results are presented in Figure 6, a graph of the number average and weight average molecular weight as a function of conversion of the limiting functional group. The asymptotic limit in the weight average molecular weight was used to approximate the critical conversion. Results tabulated in Table I1 in the column labeled “eq 16” were based on the tabulated rate constants and show that gel point predictions can be within 1 or 2% of the experimental points. When r = 1.0 and 50% and 70% solvent was present, the prediction experienced a greater error. These results were effected adversely by extrapolations. The data set used in determining the relative rate constant with 70% solvent stopped at 52% conversion, but gelation occurred at a conversion
The numerator acknowledges that there are two independent ways to form a ring with six chain segments. The denominator contains the product 6v which represents the contour length of the ringed chain that could form. The integer is the degree of polymerization for this ring. A more complex molecule will yield a series of reaction rate expressions to represent distinct rings that can form. Each term in this series will be inversely dependent on the degree of polymerization of the specific ring to the threehalf power and will be proportional to the number of ways the numerous chemical moieties can react to form it. Temple27 addressed the polymerization kinetics associated with a trifunctional and a bifunctional reactant. Numerical calculations included the fraction of all functionalities which reacted intramolecularly tr as a function of all functionalities which reacted intermolecularly a.A balanced stoichiometry was used. These two variables
Macromolecules, Vol. 26,No. 23, 1993
6162 Liu et al.
,.b
c
b
Y
'

v
k 0.0025~S
Simulation pointa, k*/kl=0.09 0 Temple's simulation points, kl/kl=O.10
j
I
I !
x
e
S h u h t i o n points, k,/k~=4.6 Temple's simuktion points, k,/kr=4.0
5
g CI
P
i 0.111 e .El 0.08
0002
Y
B
c1
1 z
.I
2
0.060.04
. I
Y
0.0005i
1 I
El
0
c
0.021
p '
. I
Y
,
r
0 1 0 1 2 0.14 0.16 018 0 2
a
Functionalities reacted intermolecularly ( 4 )
Figure 7. Fraction of functionalgroupsreacted intramolecularly us the fraction of functional groups reacted intermolecularly c f ~ = 2, f B
E
3, r = 1).
h
b u
,x 2
8 a
00351 1
03j
c SLmuktion points, k,/k1=1.8
0 Temple's aimuktion points, kr/ k , = l . 8
q I
I
m
e
0025l
3
0021
7 $
0015
.e
l
a
I
..P
0011
4
7 00051
.*El0 B
2
0
!
0
I
! > 8 , I 0.02 0 0 4 006 0.08 0 1 0 1 2 0 1 4 0 1 6 0 1 8 0 2
Functionalities reacted intermolecularly (a)
Figure 8. Fractionof functionalgroups reacted intramolecularly us the fraction of functionalgroups reacted intermolecularly c f ~ = 2, f B = 3, r = 1). can be expressed in terms of current notation: CiAxiBxjpiA,iB j CT=
~PI,o,o (0)
Simulations were for three values of the relative rate constant and demonstrated dynamic effects of intramolecular reactions. Lid3 used the simplified rate expression presented and fit Temple's simulations visually, adjusting the relative rate constant as required. Comparisons of the two numerical simulations appear in Figures 79 for the three values of the relative rate constant selected by Temple, kdkl= (kdk,)(u)3/2 = 0.10,1.8, and 4.6,respectively. The current model satisfactorily approximates Temple's simulations using the same or nearly the same relative rate constant, 0.09,1.8, and 4.6,respectively. Therefore, if the prime variables of interest are functions of the leading momenta of the distribution, the simplified intramolecular rate expression approach is a satisfactory approximation. A second consideration for selecting the simplified rate expression lies in the area of experimental measurement. The population density distribution variable PiA,igj can potentially be measured using modern fractionation
Functionalities reacted intermolecularly (a)
Figure 9. Fraction of functionalgroups reacted intramolecularly vs the fraction of functional groups reacted intermolecularly c f ~ = 2, fe = 3, r = 1). techniques, but it is very questionable if the numerous isomers of molecules at a specific chemical composition can ever be characterized. Conclusions The chemicalreaction analysis of the thermosetting resin was successful. The reaction rate expression selected for intramolecular reactions is sufficiently complex to approximate reality in a polyurethane resin up to gelation. The extent of cyclization as a function of conversion correlated data from the literature. The model is sufficiently sensitive to its environment to allow for the determination of the relative rate constant as a function of dilution, a phenomenon which is fundamentally consistent with cyclization theory. Simulations revealed that the present approach reproduces results of simulations based on fundamental, intramolecular rate expressions developed by Temple.27 A significant reduction in the dimensions of the numerical program is realized through the approximate rate expression. Temple was able to achieve conversionsof only about 0.25 using 150 equations to describe the chemical isomers that contained up to 11 monomer units and three intramolecular bonds. The current model would require only 40 equations. Greater reductions in the dimension of the simulation are achieved as degree of polymerization increases. With an increase of the maximum number of trifunctional monomer unita in amolecule to 15,the current work extented the range in conversion to the gel point. The analysis by Noureddini and Timm% reveals that for monomers that yield polymeric molecules with the same number of each chemical moiety, similar simulations could be limited to moment equations. Acknowledgment. This work was supported by the Engineering Research Center and the Center for Materials Research and Analysis, University of Nebraska. Appendix The equations describing the secondorder moments are listed in the Appendix. The equations were derived from the weighted, population density distributions, eq 5. Initial conditione equal zero, except for the moment CiACigCiiA'pi,igj(O) = PI,O,O(~).
iA
ig
j
(A1)
Macromolecules, Vol. 26, No. 23, 1993
Urethane Polymerization to Gelation 6163
References and Notes (1) Semlyen, J. A., Ed. Cyclic Polymers; Elsevier: London, 1986. (2) Jacobson, H.; Stockmayer, W. H. J. Chem. Phys. 1950,18,160. (3) Flory, P. J. Principles ofPoZymerChemistry; Cornell University Press: Ithaca, NY, 1953. (4) Stockmayer, W. H. J. Chem. Phys. 1943,11,45; 1944,12,125.
(5) Semlyen, J. A. Cyclic Polymers; Semlyen, J. A,, Ed.; Elsevier: London, 1986, p 1. (6) Mark, J. E.; Flory, P. J. J. Am. Chem. SOC. 1964,86, 138. 1964, 86, 141. (7) Crescenzi, V.; Flory, P. J. J.Am. Chem. SOC. (8) Flory, P. J.; Crescenzi, V.; Mark, J. E. J. Am. Chem. SOC. 1964, 86, 146. (9) Fluendy, M. A. D. Trans. Faraday SOC.1963,59, 1681. (10) Carmichael, J. V.; Kingsinger, J. B. Can. J. Chem. 1964, 42, 1996. (11) Semlyen, J. A. Trans. Faraday SOC. 1967,63, 2342. (12) Winnik, M. A.; Trueman, R. E.; Jackowski, G.; Saunders, D. S. J. Am. Chem. SOC. 1974,96,4843. (13) Flory, P. J.; Suter, U. W.; Mutter, M. J. Am. Chem. SOC.1976, 98,5733. (14) Suter, U. W.; Mutter, M.; Flory, P. J. J. Am. Chem. SOC. 1976, 98,5740. 1976, (15) Mutter, M.; Suter, U. W.; Flory, P. J. J. Am. Chem. SOC. 98,5745. 1977, 99, 8307. (16) Mutter, M. J. Am. Chem. SOC. (17) Gordon, M.; Scantlebury, G. R. Pr0c.R. Soc.London 1966,A292, 380. (18) Stepto, R. F. T.; Waywell, D. R. Makromol. Chem. 1972, 152, 263. (19) Gordon, M.; Temple, W. B. Makromol. Chem. 1972,152, 277. (20) Stanford, J. L.; Stepto, R. F. T.; Wayell, D. R. J. Chem. SOC., Faraday Trans. 1 1975, 71,1308. (21) Stepto, R. F. T. Faraday Discuss. Chem. SOC. 1974,57,69. (22) Gordon, M.; Temple, W. B. Makromol. Chem. 1972,160,263. (23) Noureddini, H. Kinetic Analysis of Epoxy Resins: Competing (24) (25) (26) (27) (28) (29) (30) (31) (32) (33) iA
in
i
ir
in
i (34)
Intermolecular and Intramolecular Polymerization Reactions; Ph.D. Dissertation, University of Nebraska, Lincoln, NE,1991. Fulks, W. Advanced Calculus: An Introduction t o Analysis; Wiley: New York, 1964. Shy, L. Y.; Eichinger, B. E. Br. Polym. J. 1985,17, 200. Stanford, J. L.; Stepto, R. F. T. Br. Polym. J. 1977, June, 124. Temple, W. B. Makromol. Chem. 1972,160, 277. Noureddini, H.; Timm, D. C. Macromolecules 1992,25,1725. Billmeyer, F. W., Jr. Textbook ofPolymer Science; Wiley: New York, 1984. Odian, G. Principles ofPolymerization; Wiley: New York, 1981. Stockmayer, W. H. J. Polym. Sci. 1952, ZX, No. 1,69. Fukui, K.; Yamabe, T. J. Polym. Sci. A 1964, 2, 3743. Liu, B. Kinetic Analysis of Network Resins: Aliphatic Polyurethanes; M.S. Dissertation, University of Nebraska, Lincoln, NE, 1992. Carnahan, B.; Luther, H. A.; Wilkes, J. 0. Applied Numerical Methods; Wiley: New York, 1969; p 363.